SECTION 03450 Architectural Precast Concrete · SECTION 03450 Architectural Precast Concrete PCI...
Embed Size (px)
Transcript of SECTION 03450 Architectural Precast Concrete · SECTION 03450 Architectural Precast Concrete PCI...
Issue Date 9/28/04
SECTION 03450Architectural Precast Concrete
PCI GUIDE SPECIFICATION FOR ARCHITECTURAL PRECASTCONCRETE
Guide Specification Development:
These Guide Specifications have been developed jointly by PCI, Gensler and the American Institute ofArchitects (AIA), Master Systems publishers of MASTERSPEC®.
Guide SpecificationThis Guide Specification is intended to be used as a basis for the development of an office masterspecification or in the preparation of specifications for a particular project. In either case this GuideSpecification must be edited to fit the conditions of use. Particular attention should be given to thedeletion of inapplicable provisions or inclusion of appropriate requirements. Coordinate thespecifications with the information shown on the contract drawings to avoid duplication or conflicts.
Shaded portions are Notes to the Specification Writer.
SECTION 03450 ARCHITECTURAL PRECAST CONCRETE
This Section uses the term “Architect.” Change this term to match that used to identify the designprofessional as defined in the General and Supplementary Conditions. Verify that Section titlesreferenced in this Section are correct for this Project’s Specifications; Section titles may have changed.
PART 1 – GENERAL
1.1 RELATED DOCUMENTS
A. Drawings and general provisions of the Contract, including General and Supplementary Conditionsand Division 1 Specification Sections, apply to this Section.
A. This section includes the performance criteria, materials, production, and erection of architecturalprecast concrete for the entire project. The work performed under this section includes all labor,material, equipment, related services, and supervision required for the manufacture and erection ofthe architectural precast concrete work shown on the contract drawings.
Adjust list below to suit Project. Delete paragraph below if not listing type of units.
B. This Section includes the following:1. Architectural precast concrete cladding and loadbearing units.
2. Insulated, architectural precast concrete units.3. Brick-faced, architectural precast concrete units.4. Stone-faced, architectural precast concrete units.
C. Related Sections include the following:
List below only products and construction that the reader might expect to find in this Section but arespecified elsewhere. Other sections of the specifications not referenced below, shall also apply to theextent required for proper performance of this work.
1. Division 3 Section “Cast-in-Place Concrete” for placing connection anchors in concrete.2. Division 3 Section “Glass-Fiber-Reinforced Concrete.”3. Division 4 Section “Dimension Stone Cladding” for furnishing stone facings and anchorages.4. Division 4 Section “Cast Stone” for wet or dry cast stone facings, trim, and accessories.5. Division 4 Section “Unit Masonry Assemblies” for full-thickness brick facing, mortar, and anchorages.6. Division 5 Section “Structural Steel” for connection attachment to structural-steel framing.7. Division 7 Section “Water Repellents” for water-repellent finish treatments.8. Division 7 Section “Sheet Metal Flashing and Trim” for flashing receivers and reglets.9. Division 7 Section “Joint Sealants” for elastomeric joint sealants and sealant backings.10. Division 8 Section “Aluminum Windows” for windows set into architectural precast concrete units and tiebacks for window washing equipment.
Retain paragraph below if a design reference sample has been pre-approved and is available for review.
A. Design Reference Sample: Sample of approved architectural precast concrete color, finish andtexture, pre-approved by Architect.
1.4 PERFORMANCE REQUIREMENTS
Retain this Article if delegating design responsibility for architectural precast concrete units tofabricator. AIA Document A201 requires Owner or Architect to specify performance and designcriteria.
A. Structural Performance: Provide architectural precast concrete units and connections capable ofwithstanding design loads within limits and under conditions indicated.
Retain paragraph above if placing design loads on Drawings; retain paragraph and applicablesubparagraphs below if including design loads here. Revise requirements below to suit Project, andadd other performance and design criteria if applicable.
add other performance and design criteria if applicable.
B. Structural Performance: Provide architectural precast concrete units and connections capable ofwithstanding the following design loads within limits and under conditions indicated:
As a minimum dead loads include panel weight and the weight(s) of the materials that bear on them.
1. Dead Loads: <Insert applicable dead loads.>2. Live Loads: <Insert applicable live loads.>3. Wind Loads: <Insert applicable wind loads or wind-loading criteria, positive and negative for
various parts of the building as required by applicable building code or ASCE 7, includingbasic wind speed, importance factor, exposure category, and pressure coefficient.>
4. Seismic Loads: <Insert applicable seismic design data including seismic performancecategory, importance factor, use group, seismic design category, seismic zone, siteclassification, site coefficient and drift criteria.>
5. Project Specific Loads: <Insert applicable loads.>
Show locations here or on Drawings if different movement is anticipated for different buildingelements. If preferred, change deflection limits below to ratios such as L/300 for floors and L/200 forroofs.
6. Design framing system and connections to maintain clearances at openings, to allow for fabricationand construction tolerances, to accommodate live load deflection, shrinkage and creep of primarybuilding structure, and other building movements as follows: a. Upward and downward movementof [1/2 inch (13 mm)] [3/4 inch (19 mm)] [1 inch (25 mm)].
Temperature value in first subparagraph below is suitable for most of the U.S. based on assumeddesign temperature of 70 deg. F (21 Deg. C). Revise to suit local conditions. Temperature data isavailable from National Oceanic and Atmospheric Administration at www.ncdc.noaa.gov.
7. Thermal Movements: Provide for in-plane thermal movements resulting from annual ambienttemperature changes of 80 deg F (27 deg C) <Insert temperature>. Use other values, greater orsmaller, whenever justified by climatic conditions at the projectsite.
Delete paragraph below if fire resistance rating is not required. Fire ratings depend on occupancy andbuilding construction type, and are generally a building code requirement. When required, fire-ratedproducts should be clearly identified on the design drawings.
8. Fire Resistance Rating: Select material and minimum thicknesses to provide <one hour> <twohour> fire rating.
Delete paragraph below if window washing system is not required.
9. Window Washing System: Design panels for window washing system indicated to resist forcestransmitted from window washing equipment pull-out and horizontal shear. All design criteriafor window washing system, including material and equipment, furnished by Owner.
Retain paragraph below if stone faced precast concrete are used on project.
10. Stone to Precast Anchorages: Provide anchors, as determined through Owner’s or stonesupplier testing, in numbers, types and locations as required to satisfy the performancecriteria specified, but not less than the following.a. Minimum Anchorage Requirement: Not less than 2 anchors per stone unit of less than 2
sq. ft. (0.19 sq. m) in area and 4 anchors per unit of less than 12 sq. ft. (1.1 sq. m) in areaand for units larger than 12 sq. ft. (1.1 sq. m) in area, provide anchors spaced not morethan 24 inches (600 mm) o.c. both horizontally and vertically, all located a minimum of 6inches (150 mm) from stone edge.
Delete paragraph below if units are not used in parking structure to resist impact load.
11. Vehicular Impact Loads: Design spandrel beams acting as vehicular barrier for passenger cars toresist a single load of 6,000 lbs (26.7 kN) service load and 10,000 lbs (44.5 kN) ultimate loadapplied horizontally in any direction to the spandrel beam, with anchorages or attachmentscapable of transferring this load to the structure. For design of these beams, assume the load toact at a height of 18 inches (460 mm) above the floor or ramp surface on an area not to exceed 1sq. ft. (305 mm_).
A. Product Data: For each type of product indicated. Retain quality control records and certificates ofcompliance for 5 years or period of warranty, whichever is greater.
B. Design Mixes: For each concrete mix along with compressive strength and water-absorption tests.
C. Shop (Erection) Drawings: Detail fabrication and installation of architectural precast concrete units.Indicate member locations, plans, elevations, dimensions, shapes and cross sections. Indicateaesthetic intent including joints, reveals, and extent and location of each surface finish. Indicatedetails at building corners.1. Indicate separate face and backup mix locations, and thicknesses.2. Indicate welded connections by AWS standard symbols. Detail loose and cast-in hardware, and
connections.3. Indicate locations, tolerances and details of anchorage devices to be embedded in or attached to
structure or other construction.4. Indicate locations, extent and treatment of dry joints if two-stage casting is proposed.5. Indicate plans, and/or elevations showing unit location, and sequence of erection for special
conditions.6. Indicate location of each architectural precast concrete unit by same identification mark placed
on panel.7. Indicate relationship of architectural precast concrete units to adjacent materials.8. Indicate locations and details of brick units and joint treatment.9. Indicate locations and details of stone facings, stone anchors, and joint widths.
10. Design Modifications:a. If design modifications are necessary to meet the performance requirements and field
conditions, submit design calculations and drawings. Do not adversely affect the appearance,durability or strength of units when modifying details or materials and maintain the generaldesign concept.
Retain subparagraph below if “Performance Requirements” Article is retained. Delete or modify ifArchitect assumes or is required by law to assume design responsibility.
11. Comprehensive engineering design [signed and sealed] [certified] by the qualified professionalengineer responsible for its preparation registered in the state in which the project is located.Show governing panel types, connections, and types of reinforcement, including specialreinforcement. Coordinate the location, type, magnitude and direction of all imposed loadingsfrom the precast system to the building structural frame with the Engineer of Record.
Retain paragraph below if finishes, colors, and textures are preselected, specified, or scheduled.
D. Samples: Design reference samples for initial verification of design intent, approximately 12 by 12by 2 inches (300 by 300 by 50 mm), representative of finishes, color, and textures of exposedsurfaces of architectural precast concrete units.1. When back face of precast concrete unit is to be exposed, show samples of the workmanship,
color, and texture of the backup concrete as well as the facing.
E. Samples for each brick unit required, showing the full range of color and texture expected. Supplysketch of each corner or special shape with dimensions. Supply sample showingcolor and texture of joint treatment.
Retain first paragraph below if procedures for welder certification are retained in “QualityAssurance” Article.
F. Welding Certificates: Copies of certificates for welding procedure specifications (WPS) andpersonnel.
Manufacturer should have a minimum of 2 years of production experience in architectural precastconcrete work comparable to that shown and specified, in not less than three projects of similar scopewith the Owner or Architect determining the suitability of the experience.
G. Qualification Data: For firms and persons specified in “Quality Assurance” Article to demonstratetheir capabilities and experience. Include list of completed projects with project names andaddresses, names and addresses of architects and owners, and other information specified.
Delete test reports below if not required.
H. Material Test Reports: From a qualified testing agency indicating and interpreting test results ofthe following for compliance with requirements indicated:
Retain paragraph above or below.
I. Material Certificates: Signed by manufacturers certifying that each of the following itemscomplies with requirements.
Retain list below with either paragraph above. Edit to suit Project.
1. Concrete materials.2. Reinforcing materials and prestressing tendons.3. Admixtures.4. Bearing pads.5. Structural-steel shapes and hollow structural sections.6. Insulation7. Brick units.8. Stone anchors.
17.6 QUALITY ASSURANCE
A. Erector Qualifications:
Erector should have a minimum of 2 years of experience in architectural precast concrete workcomparable to that shown and specified in not less than three projects of similar scope with the owneror Architect determining the suitability of the experience. The inclusion of erection in the precastconcrete contract should be governed by local practices. See PCI’s website www.pci.org for currentPCI-Qualified Erectors.
1. A precast concrete erector Qualified by the Precast/Prestressed Concrete Institute (PCI) prior tobeginning work at the projectsite. Submit a current Certificate of Compliance furnished by PCIdesignating qualification in [Category A (Architectural Systems) for non-load-bearingmembers] [Category S2 (Complex Structural Systems) for load-bearing members].
Retain paragraph below if PCI-Qualified Erector is not available for Project.
2. An erector with a minimum of 2 years of experience who has completed architectural precastconcrete work similar in material, design, and extent to that indicated for this Project andwhose work has resulted in construction with a record of successful in-service performance andwho meets the following requirements:a. Retains a PCI Certified Field Auditor, at erector’s expense, to conduct a field audit of a
project in the same category as this Project prior to start of erection. Submits Erectors PostAudit Declaration.
b. The basis of the audit is the “PCI Erector’s Manual - Standards and Guidelines for theErection of Precast Concrete Products” MNL 127.
B. Fabricator Qualifications: A firm that complies with the following requirements and isexperienced in producing architectural precast concrete units similar to those indicated for thisProject and with a record of successful in-service performance.
1. Assumes responsibility for engineering architectural precast concrete units to comply withperformance requirements. This responsibility includes preparation of Shop Drawings andcomprehensive engineering analysis by a qualified professional engineer.
Delete subparagraph above and below if Contractor is not required to engage the services of aqualified professional engineer and if submission of a comprehensive engineering analysis is notretained in “Submittals” Article.
2. Professional Engineer Qualifications: A professional engineer who is legally qualified topractice in jurisdiction where Project is located and who is experienced in providingengineering services of the kind indicated. Engineering services are defined as those performedfor installations of architectural precast concrete that are similar to those indicated for thisProject in material, design, and extent.
3. Participates in PCI’s Plant Certification program at the time of bidding and is designated a PCI-certified plant for Group A, Category A1- Architectural Cladding and Load Bearing Units.
4. Has sufficient production capacity to produce required units without delaying the Work.
Delete subparagraph below if fabricators are not required to be registered with and approved byauthorities having jurisdiction. List approved fabricators in Part 2 if required.
5. Is registered with and approved by authorities having jurisdiction.
Retain first paragraph below if PCI Certification Program provides quality assurance testing, andadditional quality assurance testing is required. Testing agency is normally engaged by Owner.
C. Testing Agency Qualifications: An independent testing agency, [acceptable to authorities havingjurisdiction] qualified according to ASTM C 1077 and ASTM E 329 to conduct the testingindicated, as documented according to ASTM E 548.
D. Design Standards: Comply with ACI 318 (ACI 318M) and the design recommendations of PCIMNL 120, “PCI Design Handbook – Precast and Prestressed Concrete,” applicable to types ofarchitectural precast concrete units indicated.
E. Quality-Control Standard: For manufacturing procedures and testing requirements, quality- controlrecommendations, and dimensional tolerances for types of units required, comply with PCI MNL117, “Manual for Quality Control for Plants and Production of Architectural Precast ConcreteProducts.”
Delete paragraph below if no welding is required. Retain “Welding Certificates” Paragraph in”Submittals” Article if paragraph below is retained. AWS states that welding qualifications remain ineffect indefinitely unless welding personnel have not welded for more than six months or there is aspecific reason to question their ability.
F. Welding: Qualify procedures and personnel according to AWS D1.1, “Structural Welding Code –Steel”; and AWS D1.4, “Structural Welding Code – Reinforcing Steel.”
Retain paragraph below if fire-rated units or assemblies are required. Select either PCI MNL 124 orACI 216.1/TMS 0216.1 or retain both if acceptable to authorities having jurisdiction.
ACI 216.1/TMS 0216.1 or retain both if acceptable to authorities having jurisdiction.
G. Calculated Fire-Test-Response Characteristics: Where indicated, provide architectural precastconcrete units whose fire resistance has been calculated according to [PCI MNL 124, “Design forFire Resistance of Precast Prestressed Concrete,”] [ACI 216.1/TMS 0216.1, “Standard Methodfor Determining Fire Resistance of Concrete and Masonry Construction Assemblies,”] and isacceptable to authorities having jurisdiction.
PCI recommends review of preproduction sample panels or first production unit. Revise size andnumber of sample panels to suit Project.
H. Sample Panels: After sample approval and before fabricating architectural precast concrete units,produce a minimum of two sample panels approximately 16 square feet in size for review byArchitect. Incorporate full scale details of architectural features, finishes, textures, and transitionsin the sample panels.
1. Locate panels where indicated or, if not indicated, as directed by Architect.2. Damage part of an exposed-face surface for each finish, color, and texture, and demonstrate
adequacy of repair techniques proposed for repair of surface blemishes.3. After acceptance of repair technique, maintain one sample panel at the manufacturer’s plant
and one at the projectsite in an undisturbed condition as a standard for judging the completedWork.
4. Demolish and remove sample panels when directed.
PCI recommends production of finish and texture range samples when color and texture uniformityconcerns could be an issue, the Architect or precaster has not had previous experience with thespecified mix and finish, or a large project has multiple approving authorities.
I. Range Samples: After sample panel approval and before production fabriction of architecturalprecast concrete units, produce a minimum of <three> <five> samples, approximately 16 squarefeet in size, representing anticipated range of color and texture on project’s units. Following rangesample acceptance by the Architect, maintain samples at the manufacturer’s plant as color andtexture acceptability reference.
Delete paragraph and subparagraphs below if sample panels above will suffice and the addedexpense of mockups is not required. If retaining, indicate location, size, and other details ofmockups on Drawings or by inserts. Revise wording if only one mockup is required.
J. Mockups: After sample approval but before production fabrication of architectural precastconcrete units, construct full sized mockups to verify selections made under sample Submittals andto demonstrate aesthetic effects and qualities of materials and execution. Mockup to berepresentative of the finished work in all respects including glass, aluminum framing, sealants andarchitectural precast concrete complete with all anchors, connections, flashings, and joint fillers asaccepted on the final shop drawings. Build mockups to comply with the following requirements,using materials indicated for the completed work:
Revise or delete subparagraphs below to suit Project.
1. Build mockups in the location and of the size indicated or, if not indicated, as directed byArchitect.
2. Notify Architect in advance of dates and times when mockups will be constructed.3. Obtain Architect’s approval of mockups before starting fabrication.4. In presence of Architect, damage part of an exposed face for each finish, color, and texture, and
demonstrate materials and techniques proposed for repairs to match adjacent undamagedsurfaces.
5. Maintain mockups during construction in an undisturbed condition as a standard for judging thecompleted Work.
6. Demolish and remove mockups when directed.
Retain subparagraph below if mockups are erected as part of building rather than separately andthe intention is to make an exception to the default requirement in Division 1 Section, ”QualityRequirements” for demolishing and removing mockups.
7. Approved mockups may become part of the completed Work if undamaged at the time ofSubstantial Completion.
Delete paragraph below if mockup above is to be used for Testing Mockup.
K. Testing Mockup: Provide a single full sized mockup for testing by others to the extent shown orindicated to simulate the precast and window wall assembly. Refer to Division 8 WINDOW ANDCURTAIN WALLS for requirements applicable to testing architectural precast concrete systems inconjunction with windows and window wall.
Delete below if Work of this Section is not extensive or complex enough to justify a pre-installationconference. If retaining, coordinate with Division 1.
L. Preinstallation Conference: Conduct conference at Project site to comply with requirements inDivision 1 Section “Project Management and Coordination.”
1.7 PRODUCT DELIVERY, STORAGE AND HANDLING
A. Store units with adequate dunnage and bracing and protect units to prevent contact with soil,staining, and to prevent cracking, distortion, warping or other physical damage.
B. Store units, unless otherwise specified, with non-staining, resilient supports.
C. Place stored units so identification marks are clearly visible, and product can be inspected.
D. Deliver all architectural precast concrete units to the project site in such quantities and at suchtimes to assure compliance with the agreed project schedule and proper setting sequence so as tolimit unloading units temporarily on the ground.
E. Handle and transport units in a position consistent with their shape and design in order to avoidexcessive stresses which would cause cracking or damage.
F. Lift and support units only at designated points shown on the Shop Drawings.
G. Place non-staining resilient spacers of even thickness between each unit.
H. Support units during shipment on non-staining shock absorbing material.
Coordination and responsibility for supply of items to be placed on or in the structure to allow place-ment of precast concrete units depends on type of structure and varies with local practice. Clearlyspecify responsibility for supply and installation of hardware. If not supplied by precast concretefabricator, supplier should be listed and requirements included in related trade sections. When thebuilding frame is structural steel, erection hardware welded to the steel frame should be supplied andinstalled as part of the structural steel. Ensure that type and quantity of hardware items to be cast intoprecast concrete units for use of other trades are specified or detailed in contract drawings andfurnished to fabricator, with instructions, in a timely manner in order not to delay the Work.
A. Furnish loose connection hardware and anchorage items to be embedded in or attached to otherconstruction without delaying the Work. Provide setting diagrams, templates, instructions, anddirections, as required, for installation.
PART 2 – PRODUCTS
Delete this Article unless naming fabricators. See PCI’s magazine “Ascent” or its Web sitewww.pci.org for current PCI-certified plant listings.
A. Available Fabricators: Subject to compliance with requirements, fabricators offering products thatmay be incorporated into the Work include, but are not limited to, the following:
Retain above for nonproprietary or below for semiproprietary specification. If above is retained,include procedure for approval of other fabricators in Instructions to Bidders. Refer to Division 1Section “Product Requirements.”
B. Fabricators: Subject to compliance with requirements, provide products by one of the following:1. <Insert fabricators’ names and product designations for acceptable manufacturers.>
2.2 MOLD MATERIALS
A. Molds: Rigid, dimensionally stable, nonabsorptive material, warp and buckle free, that willprovide continuous and true precast concrete surfaces within fabrication tolerances indicated; non-reactive with concrete and suitable for producing required finishes.1. Mold-Release Agent: Commercially produced liquid-release agent that will not bond with,
stain or adversely affect precast concrete surfaces and will not impair subsequent surface orjoint treatments of precast concrete.
Delete below if form liners are not used. Form liners may be used to achieve a special off-the-formfinish or to act as a template for thin or half brick facings. Revise to add description if particular formliner is selected.
finish or to act as a template for thin or half brick facings. Revise to add description if particular formliner is selected.
B. Form Liners: Units of face design, texture, arrangement, and configuration [indicated] [to matchprecast concrete design reference sample]. Provide solid backing and form supports to ensurethat form liners remain in place during concrete placement. Use with manufacturer’srecommended liquid-release agent that will not bond with, stain, or adversely affect precastconcrete surfaces and will not impair subsequent surface or joint treatments of precast concrete.
Delete below if not using retarder to help obtain exposed aggregate finish.
C. Surface Retarder: Chemical set retarder capable of temporarily delaying hardening of newlyplaced concrete mix to depth of reveal specified.
2.3 REINFORCING MATERIALS
Select only one of the paragraphs and subparagraphs below to suit steel reinforcement requirements.If retaining “Performance Requirements” Article, consider reviewing selections with fabricators.
A. Reinforcing Bars: ASTM A 615/A 615M, Grade 60 (Grade 420), deformed.
Retain paragraph below for reinforcement that is welded or if added ductility is sought.
B. Low-Alloy-Steel Reinforcing Bars: ASTM A 706/A 706M, deformed.
The presence of chromate film on the surface of the galvanized coating is usually visible as a lightyellow tint on the surface. ASTM B 201 describes a test method for determining the presence ofchromate coatings. Use galvanizing where corrosive environment or severe exposure conditionsjustify extra cost.
C. Galvanized Reinforcing Bars: ASTM A 767/A 767M, Class II zinc coated, hot-dip galvanized andchromate wash treated after fabrication and bending, as follows:
Select type of reinforcement to be galvanized from subparagraph below.
1. Steel Reinforcement: [ASTM A 615/A 615M, Grade 60 (Grade 420)] [ASTM A 706/A706M], deformed.
Use epoxy coating where corrosive environment or severe exposure conditions justify extra cost.ASTM A775 is a bendable coating while ASTM A934 is a non-bendable coating.
D. Epoxy-Coated Reinforcing Bars: ASTM A 775/A 775M or ASTM A 934/A 934M, as follows:
Select type of reinforcement to be epoxy coated from subparagraph below.
1. Steel Reinforcement: [ASTM A 615/A 615M, Grade 60 (Grade 420)] [ASTM A 706/A706M], deformed.
E. Steel Bar Mats: ASTM A 184/A 184M, assembled with clips, as follows:
Select type of reinforcement for mat fabrication from subparagraph below.
1. Steel Reinforcement: [ASTM A 615/A 615M, Grade 60 (Grade 420) [ASTM A 706/A706M], deformed bars.
Select only one of the paragraphs and subparagraphs below to suit steel reinforcement requirements.If retaining “Performance Requirements” Article, consider reviewing selections with fabricators.
F. Plain-Steel Welded Wire Reinforcement: ASTM A 185, fabricated from [as-drawn] [galvanizedand chromate wash treated] steel wire into flat sheets.
G. Deformed-Steel Welded Wire Reinforcement: ASTM A 497, flat sheet.
H. Epoxy-Coated-Steel Welded Wire Reinforcement: ASTM A 884/A 884M Class A coated, [plain][deformed], flat sheet, [Type 1 bendable coating] [Type 2 non-bendable coating].
I. Supports: Suspend reinforcement from back of mold or use bolsters, chairs, spacers, and otherdevices for spacing, supporting, and fastening reinforcing bars and welded wire reinforcement inplace according to PCI MNL 117.
2.4 PRESTRESSING TENDONS
Retain this Article if precast concrete units will be prestressed, either pre-tensioned or post-tensioned. ASTM A 416/A 416M establishes low-relaxation strand as the standard
A. Prestressing Strand: ASTM A 416/A 416M, Grade 270 (Grade 1860), uncoated, 7-wire, low-relaxation strand.
B. Unbonded Post-Tension Strand: ASTM A416/A416M with corrosion inhibitor conforming toASTM D1743, Grade 270 (Grade 1860), 7-wire, low-relaxation strand with polypropylene conduitsheath.
2.5 CONCRETE MATERIALS
Delete materials below not required. Revise to suit Project.
A. Portland Cement: ASTM C150, Type I or III.
Select portland cement color from options in subparagraph below. Mixing with white cement willimprove color uniformity of gray cement. White cement has greater color consistency than graycement and should be used for pastel colors. For darker colors, the variations of gray cement haveless effect on the final color hue.
1. For surfaces exposed to view in finished structure, use [gray] [and] [white], same type, brand,and mill source throughout the precast concrete production.
2. Standard gray Portland cement may be used for non-exposed backup concrete.
B. Supplementary Cementitious Materials.
Select mineral or cementitious admixtures from four paragraphs below. Where appearance is animportant factor, it is recommended that fly ash, silica fume and ground slag not be permitted.
1. Fly Ash Admixture: ASTM C 618, Class C or F with maximum loss on ignition of 3 percent.2. Metakaolin Admixture: ASTM C 618, Class N.3. Silica Fume Admixture: ASTM C 1240 with optional chemical and physical requirement.4. Ground Granulated Blast-Furnace Slag: ASTM C989, Grade 100 or 120.
ASTM C 33 limits deleterious substances in coarse aggregate depending on climate severity and in-service location of concrete. Class 5S is the most restrictive designation for architectural concreteexposed to severe weathering. PCI MNL 117 establishes stricter limits on deleterious substances forfine and coarse aggregates.
B. Normal-Weight Aggregates: Except as modified by PCI MNL 117, ASTM C 33, with coarseaggregates complying with Class 5S. Provide and stockpile fine and coarse aggregates for eachtype of exposed finish from a single source (pit or quarry) for entire project.
Revise subparagraph below and add descriptions of selected coarse- and fine-face mix aggregatecolors, sizes, and sources if required.
1. Face-Mix Coarse Aggregates: Selected, hard, and durable; free of material that reacts withcement or causes staining; to match selected finish sample.
Retain one option from first subparagraph below or insert gradation and maximum aggregate size ifknown. Fine and coarse aggregates are not always from same source.
a. Gradation: [Uniformly graded] [Gap graded] [To match design reference sample].
2. Face-Mix Fine Aggregates: Selected, natural or manufactured sand of the same material ascoarse aggregate, unless otherwise approved by Architect.
Delete paragraph below when architectural requirements dictate that face-mix be used throughout.
C. Backup Concrete Aggregates: ASTM C33 or C330.
Lightweight aggregates in a face-mix are not recommended in cold or humid climates (if exposed tothe weather) unless their performance has been verified by tests or records of previous satisfactoryusage in similar environments. If normal-weight aggregates are used in face-mix, lightweightaggregates in backup are not recommended due to bowing potential.
D. Lightweight Aggregates: Except as modified by PCI MNL 117, ASTM C 330 with absorption lessthan 11 percent.
Delete first paragraph below if coloring admixture is not required. Add color selection if known.E. Coloring Admixture: ASTM C 979, synthetic or natural mineral-oxide pigments or colored water-
reducing admixtures, temperature stable and non-fading.
F. Water: Potable; free from deleterious material that may affect color stability, setting, or strength ofconcrete and complying with chemical limits of PCI MNL 117.
Delete paragraph below if air entrainment is not required. Air entrainment should be required toincrease resistance to freezing and thawing where environmental conditions dictate.
G. Air Entraining Admixture: ASTM C 260, certified by manufacturer to be compatible with otherrequired admixtures.
Add types of chemical admixtures, if known, or limit types if required. Water-reducing admixtures,Types A, E, and D, or a high-range water reducer, Type F, predominate.
H. Water-Reducing Admixture: ASTM C 494/C494M, Type A.
I. Retarding Admixture: ASTM C 494/C494M, Type B.
J. Water-Reducing and Retarding Admixture: ASTM C 494/C494M, Type D.
K. High-Range, Water-Reducing Admixture: ASTM C 494/C494M, Type F.
L. High-Range, Water-Reducing and Retarding Admixture: ASTM C 494/C494M, Type G.
M. Plasticizing Admixture for Flowable Concrete: ASTM C 1017/C1017M.
N. Admixtures containing calcium chloride, or more than 0.15 percent chloride ions or other salts byweight of admixture are not permitted.
2.6 STEEL CONNECTION MATERIALS
Edit this Article to suit Project. Add other materials as required.
A. Carbon-Steel Shapes and Plates: ASTM A 36/A 36M except silicon (Si) content in the range of 0to 0.03% or 0.15 to 0.25% for materials to be galvanized. Steel with chemistry conforming to theformula Si + 2.5P < 0.09 is also acceptable.
B. Carbon-Steel Headed Studs: ASTM A 108, Grades 1018 through 1020, cold finished and bearingthe minimum mechanical properties for studs as indicated under MNL 117, Table 3.2.3.; AWSD1.1, Type A or B, with arc shields.
C. Carbon-Steel Plate: ASTM A 283/A 283M.
D. Malleable Iron Castings: ASTM A 47/A 47M. Grade 32510 or 35028.
E. Carbon-Steel Castings: ASTM A 27/A 27M, Grade U-60-30 (Grade 415-205).
F. High-Strength, Low-Alloy Structural Steel: ASTM A 572/A 572M except silicon (Si) content inthe range of 0 to 0.03% or 0.15 to 0.25% for materials to be galvanized. Steel with chemistryconforming to the formula Si + 2.5P < 0.09 is also acceptable.
G. Carbon-Steel Structural Tubing: ASTM A 500, Grade B.
H. Wrought Carbon-Steel Bars: ASTM A 675/A 675M, Grade 65 (Grade 450).
I. Deformed-Steel Wire or Bar Anchors: ASTM A 496 or ASTM A 706/A 706M.
ASTM A 307 defines the term “studs” to include stud stock and threaded rods.
J. Carbon-Steel Bolts and Studs: ASTM A 307, Grade A (ASTM F 568M, Property Class 4.6)carbon-steel, hex-head bolts and studs; carbon-steel nuts (ASTM A563/A563M, Grade A); and flat,unhardened steel washers (ASTM F844).
High-strength bolts are used for friction-type connections between steel members and are notrecommended between steel and concrete since concrete creep and crushing of concrete during bolttightening reduce effectiveness.
K. High-Strength Bolts and Nuts: ASTM A 325/A 325M or ASTM A490/A490M, Type 1, heavy hexsteel structural bolts, heavy hex carbon-steel nuts, (ASTM A563/A563M) and hardened carbon-steel washers (ASTM F436/F436M).
Retain paragraph and subparagraph below if galvanized finish is required. Revise locations ofgalvanized items if required. Field welding should generally not be permitted on galvanizedelements, unless the galvanizing is removed or acceptable welding procedures are submitted. Hot-dip galvanized finish provides greater corrosion resistance than electrodeposited zinc coating.Electrodeposition is usually limited to threaded fasteners.
L. Finish: For exterior steel items and items indicated for galvanizing, apply zinc coating by [hot-dipprocess according to ASTM A 123/A 123M, after fabrication, or ASTM A 153/A 153M, asapplicable] [electrodeposition according to ASTM B 633, SC 3, Type 1and 2].1. Galvanizing Repair Paint: High-zinc-dust-content paint with dry film containing not less than
94 percent zinc dust by weight, and complying with DOD-P-21035A or SSPC-Paint 20.
Retain paragraph below if paint finish is required. Revise locations of priming, if required. MPI 79(FS TT-P-664) in first option below provides some corrosion protection while SSPC-Paint 25,without topcoating, provides minimal corrosion protection.
M. Shop-Primed Finish: Prepare surfaces of non-galvanized steel items, except those surfaces to beembedded in concrete, according to requirements in SSPC-SP 1 followed by SSPC-SP 3 and shop-apply [lead- and chromate-free, rust –inhibitive primer, complying with performancerequirements in MPI 79] [SSPC-Paint 25] according to SSPC-PA 1.
N. Welding Electrodes: Comply with AWS standards.
2.7 STAINLESS-STEEL CONNECTION MATERIALS
Delete this Article if not required. Use when resistance to staining merits extra cost in parkingstructures and other high moisture or corrosive areas.
A. Stainless-Steel Plate: ASTM A 666, Type 304, of grade suitable for application.
B. Stainless-Steel Bolts and Studs: ASTM F 593, alloy 304 or 316, hex-head bolts and studs;stainless-steel nuts; and flat, stainless steel washers. Lubricate threaded parts of stainless steelbolts with an anti-seize thread lubricant during assembly.
C. Stainless-Steel Headed Studs: ASTM A 276 and bearing the minimum mechanical properties forstuds as indicated under MNL 117, Table 3.2.3.
2.8 BEARING PADS AND OTHER ACCESSORIES
Delete this Article if not applicable. Choice of bearing pad can usually be left to fabricator;coordinate selection with structural engineer if required.
A. Provide bearing pads for architectural precast concrete units as follows:1. Elastomeric Pads: AASHTO M 251, plain, vulcanized, 100 percent polychloroprene
(neoprene) elastomer, molded to size or cut from a molded sheet, 50 to 70 Shore A durometeraccording to ASTM D2240, minimum tensile strength 2250 psi (15.5 MPa) per ASTM D 412.
2. Random-Oriented, Fiber-Reinforced Elastomeric Pads: Preformed, randomly orientedsynthetic fibers set in elastomer. Surface hardness of 70 to 90 Shore A durometer according toASTM D2240. Capable of supporting a compressive stress of 3000 psi (20.7 MPa) with nocracking, splitting or delaminating in the internal portions of the pad. Test one specimen foreach 200 pads used in the project.
3. Cotton-Duck-Fabric-Reinforced Elastomeric Pads: Preformed, horizontally layered cotton-duck fabric bonded to an elastomer. Surface hardness of 80 to 100 Shore A durometeraccording to ASTM D2240. Conforming to Division II, Section 18.10.2 of AASHTO LRFDBridge Design Specifications, or Military Specification, MIL-C-882D.
4. Frictionless Pads: Tetrafluoroethylene (teflon), glass-fiber reinforced, bonded to stainless ormild-steel plates, of type required for in-service stress.
5. High-Density Plastic: Multimonomer, nonleaching, plastic strip.
Select material from options in paragraph below or add another material to suit Project. Coordinatewith counterflashing materials and details.
B. Reglets: [PVC extrusions.] [Stainless steel, Type 302] [Copper] [Reglets and flashing arespecified in Division 7 Section “Sheet Metal Flashing and Trim.”] felt or fiber filled or coverface opening of slots.
C. Accessories: Provide clips, hangers, plastic or steel shims, and other accessories required to installarchitectural precast concrete units.
2.9 GROUT MATERIALS
Add other proprietary grout systems to suit Project. Show locations of each grout here or onDrawings if more than one type is retained.
A. Sand-Cement Grout: Portland Cement, ASTM C 150, Type I, and clean, natural sand, ASTM C144, or ASTM C 404. Mix at ratio of 1 part cement to 2-1/2 parts sand, by volume, with minimumwater required for placement and hydration.
Retain paragraph below if nonshrink grout is required or if cement-grout shrinkage could causestructural deficiency. For critical installations, require manufacturer to provide field supervision.
B. Nonmetallic, Nonshrink Grout: Premixed, nonmetallic, noncorrosive, nonstaining grout containingselected silica sands, portland cement, shrinkage-compensating agents, plasticizing and water-reducing agents, complying with ASTM C 1107, Grade A for drypack and Grades B and C forflowable grout and of a consistency suitable for application within a 30-minute working time.
C. Epoxy-resin grout: Two-component mineral-filled epoxy-resin: ASTM C881 of type, grade, andclass to suit requirements.
2.10 THIN AND HALF BRICK UNITS AND ACCESSORIES
Retain this Article if specifying thin veneer brick-faced precast concrete panels. Type TBX brickunits feature the tightest dimensional tolerances but may be too dimensionally variable to fitsecurely within form liner templates. Pre-select brick and name prior to bid or establish set costallowance. If full-size brick units are required, use Division 4 Section “Unit Masonry Assemblies.”
A. Thin or Half Brick Units: ASTM C216, Type FBX or ASTM C 1088, Grade Exterior, Type TBX,[not less than _ inch (13 mm)] [3/4 inch (19 mm)] [1 inch (25 mm)] thick with a tolerance ofplus or minus 1/16 inch (1.59 mm) and as follows:1. Face Size: Standard, 2-1/4 inches (57 mm) high by 8 inches (203 mm) long.2. Face Size: Modular, 2-1/4 inches (57 mm) high by 7-1/2 to 7-5/8 inches (190 to 194 mm) long.3. Face Size: Engineer Modular, 2-3/4 to 2-13/16 inches (70 to 71 mm) high by 7-1/2 to 7-5/8
inches (190 to 194 mm) long.4. Face Size: Closure Modular, 3-1/2 to 3-5/8 inches (89 to 92 mm) high by 7-1/2 to 7-5/8 inches
(190 to 194 mm) long.5. Face Size: Utility, 3-1/2 to 3-5/8 inches (89 to 92 mm) high by 11-1/2 to 11-5/8 inches (292 to
295 mm) long.6. [Where shown to “match existing,”] provide face brick matching color, texture, and face size
of existing adjacent brickwork.a. <Insert information on existing brick if known.>
Select from subparagraphs above face sizes with equivalent metric dimensions or fromsubparagraphs below for products manufactured to metric face sizes. If retaining below, verifyavailability of sizes.
7. Face Size: Metric modular, 57 mm high by 190 mm long.8. Face Size: Metric engineer, 70 mm high by 190 mm long.9. Face Size: Metric closure, 90 mm high by 190 mm long.10. Face Size: Metric utility, 90 mm high by 290 mm long.
Show details on Drawings of special conditions and shapes if required.
11. Special Shapes: Include corners, edge corners, and end edge corners.
Thin brick units with higher rates of absorption than values in first subparagraph below should bewetted before placing concrete to improve bond. Before retaining paragraph, verify that thin brickselected complies with requirements.
12. Initial Rate of Absorption: Less than 30g/30 sq. in. (30g/194 sq. cm.) per minute when testedper ASTM C 67.
13. Efflorescence: Provide brick that has been tested according to ASTM C 67 and is rated “noteffloresced.”
Delete subparagraph below if surface-colored brick is not used.
14. Surface Coloring: Brick with surface coloring, other than flashed or sand-finished brick, shallwithstand 50 cycles of freezing and thawing per ASTM C 67 with no observable difference inthe applied finish when viewed from 10 feet (3 m).
Options in subparagraph below are examples of descriptive requirements for appearance where aproprietary specification cannot be used. If approving a color range for brick, view 100 square feetof loose bricks or a completed building. Edit to suit Project or delete if brick is specified by productname.
15. Face Color and Texture: [Match Architect’s samples] [Medium brown, wire cut] [Full-range red, sand molded] [Gray, velour].
Retain first subparagraph below, deleting inapplicable descriptions if required.
16. Back Surface Texture: Scored, combed, wire roughened, ribbed, keybacked or dovetailed.17. Available Products: Subject to compliance with requirements, products that may be
incorporated into the Work include, but are not limited to, the following:
Retain subparagraph above for nonproprietary or subparagraph below for semiproprietarySpecification. Refer to Division 1 Section “Materials and Equipment.”
18. Products: Subject to compliance with requirements, provide one of the following:
a. <Insert manufacturers’ names and product designations for acceptable face brick.>
Refer to American National Standards Institute (ANSI) A 137.1 for the commonly available sizesand shapes, physical properties, the basis for acceptance and methods of testing.
B. Glazed and Unglazed Ceramic Tile Units: ANSI A 137.1 [not less than 3/8 inch (10 mm)]1. Body of glazed tile shall have a water absorption of less than 3 percent using ASTM C373.2. Manufacturer shall warrant materials as frost-resistant.3. Glazed units shall conform to ASTM C126.
C. Architectural Terra Cotta Units: Comply with requirements of Architectural Terra Cottamanufacturers’ standards for the application indicated.
Retain paragraph below if mortar setting brick unit joints before placing precast concrete mix.
D. Setting Mortar: Portland cement, ASTM C 150, Type I, and clean, natural sand, ASTM C 144.Mix at ratio of 1 part cement to 4 parts sand, by volume, with minimum water required forplacement.
Delete paragraph and subparagraphs below if not filling thin brick unit joints with pointing groutafter precast concrete panel production.
E. Latex-Portland Cement Pointing Grout: ANSI A118.6 and as follows:
Select one or both types of grout from first two subparagraphs below.
1. Dry-grout mixture, factory prepared, of portland cement, graded aggregate, and dry,redispersible, ethylene-vinyl-acetate additive for mixing with water; uniformly colored.
2. Commercial portland cement grout, factory prepared, with liquid styrene-butadiene rubber oracrylic-resin latex additive; uniformly colored.
3. Colors: [As indicated by manufacturer’s designations] [Match Architect’s samples] [Asselected by Architect from manufacturer’s full range].
F. Setting Systems
Retain paragraphs below if thin brick, ceramic tile, or full brick will be laid after casting of panel.
1. Thin brick and Ceramic Tile Units: [Dry-Set Mortar: ANSI A118.1] [Latex-Portland Cement Mortar: ANSI A 118.4]2. Full Brick Units: Install <Galvanized> <Type 304 stainless steel> dovetail slots in precast:
not less than 0.5 mm thick, felt or fiber filled or cover face opening of slots. Attach brick units with wire anchors, ASTM A82 or B227, Grade 30HS not less than 3/16 inch (W2.8) in diameter and hooked on one end and looped through a 7/8 in. (25 mm) wide, 12-gage (2.68 mm) steel sheet bent over the wire with dovetail on opposite end.
2.11 STONE MATERIALS AND ACCESSORIES
Retain this Article if stone facing is required. Material, fabrication, and finish requirements areusually specified in Division 4 Section “Dimension Stone Cladding.” Replace first paragraph belowwith stone requirements, if preferred.
usually specified in Division 4 Section “Dimension Stone Cladding.” Replace first paragraph belowwith stone requirements, if preferred.
A. Stone facing for architectural precast concrete is specified in Division 4 Section “Dimension StoneCladding.”1. Tolerance of length and width of +0, -1/8 inch (+0, -3mm).
Anchors are generally supplied by stone fabricator or, in some cases, by precaster. Specify supplier.Anchors may be toe-in, toe-out, or dowels.
B. Anchors: Stainless steel, ASTM A 666, Type 304, of temper and diameter required to supportloads without exceeding allowable design stresses.
Grommets will usually be required if filling dowel holes with rigid epoxy.
1. Fit each anchor leg with 60 durometer neoprene grommet collar of width at least twice thediameter and of length at least five times the diameter of the anchor.
C. Sealant Filler: ASTM C 920, low-modulus, multicomponent, nonsag urethane sealant complyingwith requirements in Division 7 Section ”Joint Sealants” and that is nonstaining to stone substrate.
Dowel hole filling is used to prevent water intrusion into stone and future discoloration at anchorlocations. Retain paragraph above for a flexible filler or paragraph below for a rigid filler.
D. Epoxy Filler: ASTM C 881, 100 percent solids, sand –filled non-shrinking, non -staining of type,class, and grade to suit application.
E. Bond Breaker:1. Preformed, compressible, resilient, nonstaining, nonwaxing, closed-cell polyethylene foam pad,
nonabsorbent to liquid and gas, 1/8 inch (3.2 mm) thick.2. Polyethylene sheet, 6 to 10 mil thick.
2.12 INSULATED PANEL ACCESSORIES
Retain this Article if insulated, architectural precast concrete panels are required. State desiredminimum aged R-value or thickness required, or both. Select insulation material from one of thethree following paragraphs; if using more then one type identify location.
A. Expanded-Polystyrene Board Insulation: Rigid, cellular polystyrene thermal insulation complyingwith ASTM C578 formed by expansion of polystyrene base resin; <square edges> <ship-lapedges>; with R-value of <state value> and thickness of <state thickness>.
B. Extruded-Polystyrene Board Insulation: Rigid cellular polystyrene thermal insulation complyingwith ASTM C578 formed from polystyrene base by an extrusion process; <square edges> <ship-lap edges>; with R-value of <state value> and thickness of <state thickness>.
C. Polyisocyanurate Board Insulation: Rigid, cellular polyisocyanurate thermal insulation; complying with ASTM C 591; square edged; with R-value of <state value> and thickness of <state thickness>.
Select wythe connectors from paragraph below.
D. Wythe Connectors: <Glass-fiber and vinyl-ester polymer connectors>, <polypropylene pin connectors>, <stainless-steel pin connectors>, <bent galvanized reinforcing bars or galvanized welded wire trusses>, <cylindrical metal sleeve anchors>, manufactured to connect wythes of precast concrete panels.
2.13 CONCRETE MIXES
A. Prepare design mixes to match Architect’s sample for each type of concrete required.
Revise subparagraph below if fly ash, blast furnace slag, or silica fume are not permitted. Revisepercentage to suit Project.
1. Limit use of fly ash and granulated blast-furnace slag to 20 percent replacement of portland cement by weight; metakaolin and silica fume to 10 percent of portland cement by weight.
B. Design mixes may be prepared by a qualified independent testing agency or by qualified precastplant personnel at architectural precast concrete fabricator’s option.
C. Limit water-soluble chloride ions to the maximum percentage by weight of cement permitted byACI 318 (ACI 318M) or PCI MNL 117 when tested in accordance with ASTM C1218/C1218M.
Architectural precast concrete units may be manufactured with a separate “architectural” face mixand a “structural” backup mix. Face and backup mixes should have similar shrinkage and expansioncoefficients. Similar water-cementitious materials ratios and cement-aggregate ratios arerecommended to limit bowing or warping.
D. Normal-Weight Concrete Face and Backup Mixes: Proportion mixes by either laboratory trialbatch or field test data methods according to ACI 211.1, with materials to be used on project, toprovide normal-weight concrete with the following properties:
Retain subparagraph below or revise to suit Project. Higher-strength mixes may be available; verifywith fabricators.
1. Compressive Strength (28 Days): 5000 psi (34.5 MPa).
A water-cementitious materials ratio of 0.40 to 0.45 is usual for architectural precast concrete.Lower ratios may be possible with use of high-range water reducers. Revise ratio as required.
2. Maximum Water-Cementitious Materials Ratio: 0.45.
Water absorption indicates susceptibility to weather staining. The limit in paragraph below,corresponding to 6 percent by weight, is suitable for average exposures. Different parts of a singlepanel cannot be produced with different absorptions. Verify that fabricator can produce units withlower water absorption because special consolidation techniques to increase concrete density arerequired.
E. Water Absorption: 6 percent by weight or 14 percent by volume, tested according to PCI MNL117.
Lightweight backup mixes must be compatible with normal-weight face mixes to minimize bowingor warping. Retain lightweight concrete backup mixes if required or as an option if satisfactorydurability and in-service performance are verified by fabricator.
F. Lightweight Concrete Backup Mixes: Proportion mixes by either laboratory trial batch or field testdata methods according to ACI 211.2, with materials to be used on Project, to provide lightweightconcrete with the following properties:
Retain subparagraph below or revise to suit Project. Higher-strength mixes may be available; verifywith fabricators.
1. Compressive Strength (28 Days): 5000 psi (34.5 MPa).
Increase or decrease unit weight as required. Coordinate with lightweight-aggregate supplier andarchitectural precast concrete fabricator. Lightweight concretes with lightweight and normal-weightaggregate in mix will usually be heavier than unit weight below.
2. Unit Weight: Calculated equilibrium unit weight of 115 lb/cu.ft. (1842 kg/cu.m), plus or minus3 lb/cu.ft. (48 kg/cu.m), according to ASTM C 567.
G. Add air-entraining admixture at manufacturer’s prescribed rate to result in concrete at point ofplacement having an air content complying with PCI MNL 117.
H. When included in design mixes, add other admixtures to concrete mixes according tomanufacturer’s written instructions.
2.14 MOLD FABRICATION
A. Molds: Accurately construct molds, mortar tight, of sufficient strength to withstand pressures dueto concrete-placement and vibration operations and temperature changes and for prestressing anddetensioning operations. Coat contact surfaces of molds with release agent before reinforcement isplaced. Avoid contamination of reinforcement and prestressing tendons by release agent.
Delete form liners unless needed to produce exposed surface finish.
1. Place form liners accurately to provide finished surface texture indicated. Provide solidbacking and supports to maintain stability of liners during placing of concrete. Coat form linerwith form-release agent.
B. Maintain molds to provide completed architectural precast concrete units of shapes, lines, anddimensions indicated, within fabrication tolerances specified.1. Form joints are not permitted on faces exposed to view in the finished work.
Select one option from below; show details on Drawings or revise description to add dimensions.Sharp edges or corners of precast concrete units are vulnerable to chipping.
2. Edge and Corner Treatment: Uniformly [chamfered] [radiused].
2.15 THIN AND HALF BRICK FACINGS
Retain this Article if using thin or half brick facings on architectural precast concrete units.
A. Place form liner templates accurately to provide grid for brick facings. Provide solid backing andsupports to maintain stability of liners while placing bricks and during placing of concrete.
B. Securely place brick units face down into form liner pockets and place precast concrete backingmix.
C. Clean faces and joints of brick facing.
2.16 STONE FACINGS
Retain this Article if stone facing is required. Refer to Division 4 Section “Dimensional StoneCladding” for precast veneer.
A. Accurately position stone facings to comply with requirements. Install spring clips, anchors,supports, and other attachments indicated or necessary to secure stone in place. Set stone facingsaccurately, in locations indicated on Shop Drawings. Orient stone veining in direction indicated onShop Drawings. Keep reinforcement a minimum of _ inch (19 mm) from the back surface ofstone. Use continuous spacers to obtain uniform joints of widths indicated and with edges andfaces aligned according to established relationships and indicated tolerances. Ensure no passage ofprecast matrix to stone surface.
B. See Division 7 Section “Joint Sealants” for furnishing and installing sealant backings and sealantinto stone-to-stone joints and stone-to-concrete joints. Apply a continuous sealant bead along bothsides and top of precast panels at the stone/precast interface using the bond breaker as a joint fillerback-up. Do not seal panel bottom edge.
Retain one of two subparagraphs below if sealing dowel holes. Use sealant if a flexible filler isrequired; use epoxy if a rigid filler is required.
1. Fill anchor holes with low modulus polyurethane sealant filler and install anchors.2. Fill anchor holes with epoxy filler and install anchors with _ inch (13 mm) long 60 durometer
elastomeric sleeve at the back surface of the stone.
PCI recommends preventing bond between stone facing and precast concrete to minimize bowing,cracking, and staining of stone. Retain one of two subparagraphs below.
3. Install 6 to 10 mil polyethylene sheet to prevent bond between back of stone facing andconcrete substrate.
4. Install 1/8 inch (3 mm) polyethylene-foam bond breaker to prevent bond between back of stonefacing and concrete substrate. Maintain minimum projection requirements of stone anchorsinto concrete substrate.
PCI recommends anchor spacing be determined prior to bidding. Retain below if precaster is totest stone anchors for shear and tension. ASTM E488 is preferred as ASTM C1354 does notinclude the influence of the precast concrete backup.
C. Stone Anchor Shear and Tensile Testing: Engage a certified testing laboratory acceptable to theArchitect to evaluate and test the proposed stone anchorage system. Test for shear and tensilestrength of proposed stone anchorage system in accordance with ASTM E 488 or ASTM C 1354modified as follows:
1. Prior to testing, submit for approval a description of the test assembly (including pertinent dataon materials), test apparatus and procedures.
2. Test 12-by-12 inch (300 by 300 mm) samples of stone affixed to testing apparatus throughproposed anchorages. Provide 2 sets of 6 stone samples each. One set for shear load testingand the other set for tensile load testing.
3. Test stone anchors of the sizes and shapes proposed for the installation.a. Test the assembly to failure and record the test load at failure. Record the type of failure, anchor pull-out or stone breakage, and any other pertinent information, in accordance with the requirements of ASTM E 488. In addition, submit load deflection curves of each test assembly.
D. Minimum Anchor Spacing: Anchor spaced not less than 6 inches (152 mm) from an edge with notmore than 24 to 30 inches (610 to 760 mm) between anchors depending on the local building codeand wind loading.
A. Cast-in Anchors, Inserts, Plates, Angles, and Other Anchorage Hardware: Fabricate anchoragehardware with sufficient anchorage and embedment to comply with design requirements.Accurately position for attachment of loose hardware and secure in place during precastingoperations. Locate anchorage hardware where it does not affect position of main reinforcement orconcrete placement.1. Weld headed studs and deformed bar anchors used for anchorage according to AWS D1.1 and
AWS C5.4, “Recommended Practices for Stud Welding.”
Coordinate paragraph below with Division 5 Section “Metal Fabrications” for furnishing andinstalling loose hardware items.
B. Furnish loose hardware items including steel plates, clip angles, seat angles, anchors, dowels,cramps, hangers, and other hardware shapes for securing architectural precast concrete units tosupporting and adjacent construction.
C. Cast-in reglets, slots, holes, and other accessories in architectural precast concrete units asindicated on contract drawing.
Delete first paragraph below if not applicable.
D. Cast-in openings larger than 10 inches (250 mm) in any dimension. Do not drill or cut openings orprestressing strand without approval of Architect.
E. Reinforcement: Comply with recommendations in PCI MNL 117 for fabrication, placing, andsupporting reinforcement.
1. Clean reinforcement of loose rust and mill scale, earth, and other materials that reduce ordestroy the bond with concrete. When damage to epoxy coated reinforcing exceeds limitsspecified ASTM A775/A775M repair with patching material compatible with coating materialand epoxy coat bar ends after cutting.
2. Accurately position, support, and secure reinforcement against displacement during concrete-placement and consolidation operations. Completely conceal support devices to preventexposure on finished surfaces.
3. Place reinforcing steel and prestressing strand to maintain at least 3/4 -inch (19 mm) minimumconcrete cover. Increase cover requirements for reinforcing steel to 1-1/2 inches (38 mm)when units are exposed to corrosive environment or severe exposure conditions. Arrange,space, and securely tie bars and bar supports to hold reinforcement in position while placingconcrete. Direct wire tie ends away from finished, exposed concrete surfaces.
4. Install welded wire reinforcement in lengths as long as practicable. Lap adjoining pieces atleast one full mesh spacing and wire tie laps, where required by design. Offset laps ofadjoining widths to prevent continuous laps in either direction.
F. Reinforce architectural precast concrete units to resist handling, transportation, and erectionstresses.
Delete paragraph and subparagraph below if prestressed architectural precast concrete units are notrequired. Option to prestress may be left to fabricator if objective is to aid handling and to controlcracking of units during installation.
G. Prestress tendons for architectural precast concrete units by either pretensioning or post-tensioningmethods. Comply with PCI MNL 117.
Revise release or post-tensioning strength in subparagraph below to an actual compressive strengthif required. A release strength as low as 2500 psi (17.2 MPa) for normal-weight concrete and 3000psi (20.7 MPa) for lightweight concrete is permitted.
1. Delay detensioning or post-tensioning of prestressed architectural precast concrete units untilconcrete has reached its indicated minimum design release compressive strength as establishedby test cylinders cured under the same conditions as concrete member.
2. Detension pretensioned tendons either by gradually releasing tensioning jacks or by heat-cutting tendons, using a sequence and pattern to prevent shock or unbalanced loading.
3. If concrete has been heat cured, detension while concrete is still warm and moist to avoiddimensional changes that may cause cracking or undesirable stresses.
4. Protect strand ends and anchorages with bituminous, zinc-rich or epoxy paint to avoidcorrosion and possible rust spots.
H. Mix concrete according to PCI MNL 117 and requirements in this Section. After concretebatching, no additional water may be added.
Retain paragraph below if a separate face mix is required or is Contractor’s option.
I. Place face mix to a minimum thickness after consolidation of the greater of 1 inch (25 mm) or 1.5times the maximum aggregate size, but not less than the minimum reinforcing cover as indicatedon contract drawings.1. At the fabricator’s option either of the following mix design/casting techniques may be used:
a. A single design mix throughout the entire thickness of panel.b. Design mixes for facing and backup; using cement and aggregates for each type as
indicated, for consecutive placement in the mold. Use cement and aggregate specified forfacing mix, use cement and aggregate for backup mix complying with criteria specified asselected by the fabricator.
J. Place concrete in a continuous operation to prevent seams or planes of weakness from forming inprecast concrete units. Comply with requirements in PCI MNL 117 for measuring, mixing,transporting, and placing concrete.1. Place backup concrete to ensure bond with face mix concrete.
K. Thoroughly consolidate placed concrete by internal and/or external vibration without dislocating ordamaging reinforcement and built-in items, and minimize pour lines, honeycombing or entrapped airon surfaces. Use equipment and procedures complying with PCI MNL 117.1. Place self-consolidating concrete without vibration in accordance with PCI Interim Guidelines
for the Use of Self-Consolidating Concrete.
L. Comply with ACI 306.1 procedures for cold-weather concrete placement.
M. Comply with ACI 305R recommendations for hot-weather concrete placement.
O. Identify pickup points of architectural precast concrete units and orientation in structure withpermanent markings, complying with markings indicated on Shop Drawings. Imprint orpermanently mark casting date on each architectural precast concrete unit on a surface that will notshow in finished structure.
P. Cure concrete, according to requirements in PCI MNL 117, by moisture retention without heat or by accelerated heat curing using low-pressure live steam or radiant heat and moisture. Cure units until the compressive strength is high enough to ensure that stripping does not have an effect on the performance or appearance of the final product.
Q. Repair damaged architectural precast concrete units to meet acceptability requirements of PCI MNL 117.
2.18 INSULATED PANEL CASTING
Delete this Article if integrally insulated panels are not required.
A. Cast and screed supported wythe over mold.
B. Place insulation boards, abutting edges and ends of adjacent boards. Insert wythe connectors throughinsulation, and consolidate concrete around connectors according to connector manufacturer’swritten instructions.
C. Cast and screed top wythe to meet required finish.
2.19 FABRICATION TOLERANCES
A. Fabricate architectural precast concrete units straight and true to size and shape with exposed edgesand corners precise and true so each finished unit complies with PCI MNL 117 product tolerances aswell as position tolerances for cast-in items.
Select paragraph above or paragraph and subparagraphs below. Usually retain above unless tolerancesfor Project deviate from PCI recommendations. PCI MNL 117 product tolerances, listed below, arestandardized throughout the industry. For architectural trim units such as sills, lintels, coping, cornices,quoins, medallions, bollards, benches, planters, and pavers, tolerances are listed in PCI MNL 135.
B. Fabricate architectural precast concrete units straight and true to size and shape with exposed edgesand corners precise and true so each finished unit complies with the following product tolerances.1. Overall Height and Width of Units, Measured at the Face Exposed to View: As follows:
a. 10 feet (3 m) or under, Plus or Minus 1/8 inch (3 mm).b. 10 to 20 feet (3 to 6 m), Plus 1/8 inch (3 mm), Minus 3/16 inch (5 mm).c. 20 to 40 feet (6 to 12 m), Plus or Minus 1/4 inch (6 mm).d.Each additional 10 feet (3 m), Plus or Minus 1/16 inch (1.5 mm).
2. Overall Height and Width of Units, Measured at the Face Not Exposed to View: As follows:a. 10 feet (3 m) or under, Plus or Minus 1/4 inch (6 mm).b. 10 to 20 feet (3 to 6 m), Plus _ inch (6 mm), Minus 3/8 inch (10 mm).c. 20 to 40 feet (6 to 12 m), Plus or Minus 3/8 inch (10 mm).d. Each additional 10 feet (3 m), Plus or Minus 1/8 inch (3 mm).
3. Total Thickness or Flange Thickness: Plus _ inch (6 mm), Minus 1/8 inch (3 mm).4. Rib Thickness: Plus or Minus 1/8 inch (3 mm).5. Rib to Edge of Flange: Plus or Minus 1/8 inch (3 mm).6. Distance between Ribs: Plus or Minus 1/8 inch (3 mm).7. Variation from Square or Designated Skew (Difference in Length of the Two Diagonal 8. Measurements): Plus or Minus 1/8 inch per 72 inches (3 mm per 2 m) or 1/2 inch (13 mm) total,
whichever is greater.
8. Length and Width of Block-outs and Openings within One Unit: Plus or Minus 1/4 inch (6 mm).9. Location and Dimension of Block-outs Hidden from View and Used for HVAC and Utility Penetrations: Plus or Minus 3/4 inch (19 mm).10. Dimensions of Haunches: Plus or Minus 1/4 inch (6 mm).11. Haunch Bearing Surface Deviation from Specified Plane: Plus or Minus 1/8 inch (3 mm).12 Difference in Relative Position of Adjacent Haunch Bearing Surfaces from Specified Relative Position: Plus or Minus 1/4 inch (6 mm).13. Bowing: Plus or Minus L/360, maximum 1 inch (25 mm).14. Local Smoothness: 1/4 inch per 10 feet (6 mm per 3 m).15. Warping: 1/16 inch per 12 inches (1.5 mm per 300 mm) of distance from the nearest adjacent corner.16. Tipping and Flushness of Plates: Plus or Minus 1/4 inch (6 mm).17. Dimensions of Architectural Features and Rustications: Plus or Minus 1/8 inch (3 mm).
C. Position Tolerances: For cast-in items measured from datum line location, as indicated on Shop Drawings.
1. Weld Plates: Plus or Minus 1 inch (25 mm).2. Inserts: Plus or Minus 1/2 inch (13 mm).3. Handling Devices: Plus or Minus 3 inches (75 mm).4. Reinforcing Steel and Welded Wire Reinforcement: Plus or Minus 1/4 inch (6 mm) where position has structural implications or affects concrete cover; otherwise, Plus or Minus 1/2 inch (13 mm).5. Reinforcing Steel Extending out of Member: Plus or Minus 1/2 inch (13 mm) of plan dimensions.6. Tendons: Plus or Minus 1/4 inch (6 mm), vertical; Plus or Minus 1 inch (25 mm), horizontal.7. Location of Rustication Joints: Plus or Minus 1/8 inch (3 mm).8. Location of Opening within Panel: Plus or Minus 1/4 inch (6 mm).9. Location of Flashing Reglets: Plus or Minus 1/4 inch (6 mm).10. Location of Flashing Reglets at Edge of Panel: Plus or Minus 1/8 inch (3 mm).11. Reglets for Glazing Gaskets: Plus or Minus 1/8 inch (3 mm).12. Electrical Outlets, Hose Bibs: Plus or Minus 1/2 inch (13 mm).13. Location of Bearing surface from End of Member: Plus or Minus 1/4 inch (6 mm).14. Allowable Rotation of Plate, Channel Inserts, Electrical Boxes: 2-degree rotation or 1/4 inch (6 mm) maximum over the full dimension of the unit.15. Position of Sleeve: Plus or Minus 1/2 inch (13 mm).16. Location of Window Washer Track or Buttons: Plus or Minus 1/8 inch (3 mm).
Delete paragraph below if brick faced architectural units are not used. The number of bricks allowedthese misalignments should be limited to 2 percent of the bricks on the unit.
D. Brick-Faced Architectural Precast Concrete Units. 1. Alignment of mortar joints:
a. Jog in Alignment: 1/8 inch (3 mm).b. Alignment with Panel Centerline: Plus or Minus 1/8 inch (3 mm).
2. Variation in Width of Exposed Mortar Joints: Plus or Minus 1/8 inch (9 mm).3. Tipping of Individual Bricks from the Panel Plane of Exposed Brick Surface: Plus 1/16 inch (1.5 mm); Minus 1/4 inch (6 mm) < depth of form liner joint.
4. Exposed Brick Surface Parallel to Primary Control Surface of Panel: Plus 1/4 inch (6 mm); Minus 1/8 inch (3 mm).5. Individual Brick Step in Face from Panel Plane of Exposed Brick Surface: Plus 1/16 inch (1.5mm); Minus 1/4 inch (6 mm) < depth of form liner joint.
E. Stone Veneer-Faced Architectural Precast Concrete Units.
Tolerances below are generally appropriate for smooth-finished stone. Retain, delete, or revise to suitProject.
1. Variation in Cross-Sectional Dimensions: For thickness of walls from dimensions indicated: Plus or Minus 1/4 inch (6 mm).2. Variation in Joint Width: 1/8 inch in 36 inches (3 mm in 900 mm) or a quarter of nominal joint width, whichever is less.
Revise or delete below for natural-cleft, thermal, and similar finishes.
3. Variation in Plane between Adjacent Stone Units (Lipping): 1/16 inch (1.5-mm) difference between planes of adjacent units.
A. Panel faces shall be free of joint marks, grain, and other obvious defects. Corners, including falsejoints shall be uniform, straight and sharp. Finish exposed-face surfaces of architectural precastconcrete units to match approved [design reference sample] [sample panels] [mockups] and asfollows:
This Article presumes Architect has preapproved one or more design reference samples. Includecomplete description of design reference sample here. If preapproving manufacturers, coordinate with“Manufacturers” Article. Revise if multiple samples are approved.
1. Design Reference Sample: <Insert description and identify fabricator and code number ofsample.>
Delete subparagraph below if not used. PCI published numbered, color photographs of 428 precastconcrete finishes, see PCI’s website www.pci.org. Revise below and add reference number. Addreference number combinations if more than one finish is required.
2. PCI’s “Architectural Precast Concrete –Color and Texture Selection Guide,” of plate numbersindicated.
Retain type of finish from subparagraphs below if needed. If more than one finish is required, addlocations to finish descriptions or indicate on Drawings. Add more detailed descriptions of finishesoutlined below if required when greater definition is required, such as (light), (medium), or (deep).Remove matrix to a maximum depth of one-third the average diameter of coarse aggregate but not morethan one-half the diameter of smallest sized coarse aggregate. See PCI MNL 117 for more informationon finishes. An as-cast finish generally results in a mottled surface or non-uniform finish.
on finishes. An as-cast finish generally results in a mottled surface or non-uniform finish.
3. As-Cast Surface Finish: Provide surfaces free of excessive air voids, sand streaks, andhoneycombs.
4. Textured-Surface Finish: Impart by form liners to provide surfaces free of excessive air voids,sand streaks, and honeycombs, with uniform color and texture.
5. Bushhammer Finish: Use power and hand tools to remove matrix and fracture coarse aggregates.6. Exposed Aggregate Finish: Use chemical retarding agents applied to concrete forms and
washing and brushing procedures to expose aggregate and surrounding matrix surfaces after formremoval.
7. Abrasive-Blast Finish: Use abrasive grit, equipment, application techniques, and cleaningprocedures to expose aggregate and surrounding matrix surfaces.
8. Acid-Etched Finish: Use acid and hot-water solution, equipment, application techniques, andcleaning procedures to expose aggregate and surrounding matrix surfaces. Protect hardware,connections and insulation from acid attack.
9. Honed Finish: Use continuous mechanical abrasion with fine grit, followed by filling andrubbing procedures.
10. Polished Finish: Use continuous mechanical abrasion with fine grit, followed by filling andrubbing procedures.
11. Sand-Embedment Finish: Use selected stones placed in a sand bed in bottom of mold, with sandremoved after curing.
B. Finish exposed [top] [bottom] [back] surfaces of architectural precast concrete units to match face-surface finish.
Retain paragraph above or below if applicable. Revise below to float finish or light-broom finish ifsmooth, steel-trowel finish is unnecessary.
C. Finish unexposed surfaces [top] [bottom] [and back] of architectural precast concrete units bysmooth steel-trowel finish.
Revise finish below to light-broom, stippled, or as-cast finish if float finish is unnecessary, orupgrade to smooth, steel-trowel finish.
D. Finish unexposed surfaces of architectural precast concrete units by float finish.
2.21 SOURCE QUALITY CONTROL
Always retain paragraph below because it establishes the minimum standard of plant testing andinspecting. PCI MNL 117 mandates source testing requirements and a plant Quality Systems Manual.PCI certification also ensures periodic auditing of plants for compliance with requirements in PCIMNL 117.
A. Quality-Control Testing: Test and inspect precast concrete according to PCI MNL 117 requirements.If using self-consolidating concrete also test and inspect according to PCI Interim Guidelines for theUse of Self-Consolidating Concrete.
Delete paragraph and subparagraph below if not required. PCI certification would normally beacceptable to authorities having jurisdiction without further monitoring of plant quality-control andtesting program by Owner.
B. Owner will employ an independent testing agency to verify architectural precast concrete fabricator’squality-control and testing methods.
1. Allow Owner’s testing agency access to material storage areas, concrete production equipment,concrete placement, and curing facilities. Cooperate with Owner’s testing agency and providesamples of materials and concrete mixes as may be requested for additional testing andevaluation.
C. Strength of precast concrete units will be considered deficient if units fail to comply with ACI 318(ACI 318M) requirements for concrete strength.
Review testing and acceptance criteria with structural engineer. Add criteria for load tests if required.
D. Testing: If there is evidence that the concrete strength of precast concrete units may be deficient ormay not comply with ACI 318 (ACI 318M) requirements, Precaster will employ an independenttesting agency to obtain, prepare, and test cores drilled from hardened concrete to determinecompressive strength according to ASTM C 42/C42M.1. A minimum of three representative cores will be taken from units of suspect strength, from
locations directed by Architect.2. Cores will be tested in an air-dry condition.
PCI’s recommendations below are more stringent than ACI’s.
3. Strength of concrete for each series of 3 cores will be considered satisfactory if the averagecompressive strength is equal to at least 85 percent of the 28-day design compressive strengthand no single core is less than 75 percent of the 28-day design compressive strength.
4. Test results will be made in writing on the same day that tests are performed, with copies toArchitect, Contractor, and precast concrete fabricator. Test reports will include the following:a. Project identification name and number.b. Date when tests were performed.c. Name of precast concrete fabricator.d. Name of concrete testing agency.e. Identification letter, name, and type of precast concrete units or units represented by core
tests; design compressive strength; type of break; compressive strength at breaks, correctedfor length-diameter ratio; and direction of applied load to core in relation to horizontal planeof concrete as placed.
E. Patching: If core test results are satisfactory and precast concrete units comply with requirements,clean and dampen core holes and solidly fill with precast concrete mix that has no coarse aggregate,and finish to match adjacent precast concrete surfaces.
F. Defective Work: Architectural precast concrete units that do not comply with acceptability
requirements in PCI MNL 117, including concrete strength, manufacturing tolerances, and color andtexture range are unacceptable. Chipped, spalled or cracked units may be repaired, if repaired unitsmatch the visual mock-up. The Architect reserves the right to reject any unit if it does not match theaccepted samples and visual mock-up. Replace unacceptable units with precast concrete units thatcomply with requirements.
PART 3 – EXECUTION
A. Deliver anchorage devices that are embedded in or attached to the building structural frame orfoundation before start of such work. Provide locations, setting diagrams, and templates for theproper installation of each anchorage device.
A. Examine supporting structural frame or foundation and conditions for compliance withrequirements for installation tolerances, true and level bearing surfaces, and other conditionsaffecting performance. Proceed with installation only after unsatisfactory conditions have beencorrected.
B. Do not install precast concrete units until supporting cast-in place concrete building structuralframing has attained minimum allowable design compressive strength or supporting steel or otherstructure is structurally ready to receive loads from precast.
A. Install loose clips, hangers, bearing pads and other accessories required for connecting architecturalprecast concrete units to supporting members and backup materials.
B. Erect architectural precast concrete level, plumb and square within the specified allowabletolerances. Provide temporary supports and bracing as required to maintain position, stability, andalignment of units until permanent connections are completed.
1. Install temporary steel or plastic spacing shims or bearing pads as precast concrete units arebeing erected. Tack weld steel shims to each other to prevent shims from separating.
2. Maintain horizontal and vertical joint alignment and uniform joint width as erection progresses.3. Remove projecting lifting devices and use sand-cement grout to fill voids within recessed
lifting devices flush with surface of adjacent precast concrete surfaces when recess is exposed.4. Unless otherwise shown provide for uniform joint widths of 3/4 inch (19mm)
C. Connect architectural precast concrete units in position by bolting, welding, grouting, or asotherwise indicated on approved Erection Drawings. Remove temporary shims, wedges, andspacers as soon as practical after connecting and/or grouting are completed.
1. Disruption of roof flashing continuity by connections is not permitted; concealment within roof insulation is acceptable.
D. Welding: Comply with applicable AWS D1.1 and AWS D1.4 requirements for welding, weldingelectrodes, appearance, quality of welds, and methods used in correcting welding work.
1. Protect architectural precast concrete units and bearing pads from damage by field welding orcutting operations and provide noncombustible shields as required.
2. Welds not specified shall be continuous fillet welds, using not less than the minimum fillet asspecified by AWS.
3. Clean weld affected metal surfaces with chipping hammer followed by brushing then apply aminimum 0.004 inch (100 _m) thick coat of galvanized repair paint to galvanized surfaces inconformance with ASTM A780.
Retain subparagraph above or below.
4. Clean weld affected metal surfaces with chipping hammer followed by brushing then reprimedamaged painted surfaces in accordance with manufacturer’s recommendations.
5. Visually inspect all welds critical to precast connections. Visually check all welds forcompletion and remove, reweld or repair all defective welds, if services of AWS-certifiedwelding inspector are not furnished by Owner.
E. At bolted connections, use lock washers, tack welding, or other acceptable means to preventloosening of nuts after final adjustment.
1. Where slotted connections are used, verify bolt position and tightness. For sliding connections,properly secure bolt but allow bolt to move within connection slot. For friction connectionapply specified bolt torque and check 25 percent of bolts at random by calibrated torquewrench.
Revise locations and extent of grouting in paragraph below if required.
F. Grouting Connections: Grout connections where required or indicated. Retain grout in place untilhard enough to support itself. Pack spaces with stiff grout material, tamping until voids arecompletely filled. Place grout to finish smooth, level, and plumb with adjacent concrete surfaces.Promptly remove grout material from exposed surfaces before it affects finishes or hardens.
3.4 ERECTION TOLERANCES
A. Erect architectural precast concrete units level, plumb, square, true, and in alignment withoutexceeding the noncumulative erection tolerances of PCI MNL 117, Appendix I.
Select paragraph above or paragraph and subparagraphs below. Usually retain above unlesstolerances for Project deviate from PCI recommendations. PCI MNL 117 erection tolerances arelisted below. If more exacting tolerances are required for Project, coordinate with fabricationtolerances for precast concrete as well as erection tolerances for supporting construction.
B. Erect architectural precast concrete units level, plumb, square, and true, without exceeding thefollowing noncumulative erection tolerances.
1. Plan Location from Building Grid Datum: Plus or Minus 1/2 inch (13 mm).2. Plan Location from Centerline of Steel: Plus or Minus 1/2 inch (13 mm).3. Top Elevation from Nominal Top Elevation: As follows:
a. Exposed Individual Panel: Plus or Minus 1/4 inch (6 mm).b. Nonexposed Individual Panel: Plus or Minus 1/2 inch (13 mm).c. Exposed Panel Relative to Adjacent Panel: 1/4 inch (6 mm).d. Nonexposed Panel Relative to Adjacent Panel: 1/2 inch (13 mm).
4. Support Elevation from Nominal Support Elevation: As follows:a. Maximum Low: 1/2 inch (13 mm).5. Maximum High: 1/4 inch (6 mm).
5. Maximum Plumb Variation over the Lesser of Height of Structure or 100 Feet (30 m): 1 inch(25 mm).
6. Plumb in Any 10 Feet (3 m) of Element Height: 1/4 inch (6 mm).7. Maximum Jog in Alignment of Matching Edges: 1/4 inch (6 mm).8. Joint width (Governs over Joint Taper): Plus or Minus 1/4 inch (6mm).9. Maximum Joint Taper: 3/8 inch (10 mm).10. Joint Taper in 10 Feet (3 m): 1/4 inch (6 mm).11. Maximum Jog in Alignment of Matching Faces: 1/4 inch (6 mm).12. Differential Bowing or Camber, as Erected, between Adjacent Members of Same Design: 1/4
inch (6 mm).13. Opening Height between Spandrels: Plus or Minus 1/4 inch (± 6 mm).
3.5 FIELD QUALITY CONTROL
Retain this Article if field testing and inspecting are required. Revise paragraph below if Contractorengages agency.
A. Testing: Owner will engage a qualified independent testing and inspecting agency to perform fieldtests and inspections.
B. Field welds will be subject to visual inspections and non-destructive testing in accordance withASTM E165 or ASTM E709.
C. Testing agency will report test results promptly and in writing to Contractor and Architect.
D. Repair or remove and replace work that does not comply with specified requirements.
E. Additional testing and inspecting, at Contractor’s expense, will be performed to determinecompliance of corrected work with specified requirements.
Blemishes occurring after delivery are normally repaired before final joint sealing and cleaning asweather permits.
A. Repairs will be permitted provided structural adequacy of units and appearance are not impaired.
The precast concrete manufacturer should develop appropriate repair mixtures and techniques duringthe production sample approval process.
B. Mix patching materials and repair units so cured patches blend with color, texture, and uniformityof adjacent exposed surfaces and show no apparent line of demarcation between original andrepaired work, when viewed in typical daylight illumination from a distance of 20 feet (6 m).
C. Prepare and repair damaged galvanized coatings with galvanizing repair paint according to ASTMA780.
Retain paragraph above if using galvanized anchors, connections, and other items; retain firstparagraph below if items are prime painted.
D. Wire brush, clean, and paint damaged prime-painted components with same type of shop primer.
E. Remove and replace damaged architectural precast concrete units when repairs do not meet requirements.
Specify whether erector or precaster does cleaning under the responsibility of General Contractor.
A. Clean all surfaces of precast concrete to be exposed to view, as necessary, prior to shipping.
B. Clean mortar, plaster, fireproofing, weld slag, and any other deleterious material from concretesurfaces and adjacent materials immediately.
C. Clean exposed surfaces of precast concrete units after erection and completion of joint treatment toremove weld marks, other markings, dirt, and stains.
1. Perform cleaning procedures, if necessary, according to precast concrete fabricator’srecommendations. Clean soiled precast concrete surfaces with detergent and water, using stifffiber brushes and sponges, and rinse with clean water. Protect other work from staining ordamage due to cleaning operations.
2. Do not use cleaning materials or processes that could change the appearance of exposedconcrete finishes or damage adjacent materials.
END OF SECTION 03450